1 Página 1 de 12 AASHO Road Test The AASHO Road Test, a $27 million (1960 dollars) investment and the largest road experiment of its time, was conceived and sponsored by the American Association of State Highway Officials (AASHO) as a study of the performance of highway pavement structures of known thickness under moving loads of known magnitude and frequency (Highway Research Board, 1961). The test studied both portland cement concrete and asphaltic concrete pavements, as well as certain types of short-span bridges. Major Topics on this Page Background Flexible Pavement Materials Flexible Pavement Designs Flexible Pavement Performance The information obtained from the AASHO Road Test was crucial in advancing knowledge of pavement structural design, pavement performance, load equivalencies, climate effects, and much more. The basic performance Rigid Pavement Performance information resulted in the performance equations and nomographs used in the AASHTO Guide. This section provides some background information on the AASHO Road Test. It should be helpful in understanding the experiment's strengths, weaknesses and limitations. Rigid Pavement Materials Rigid Pavement Designs Background This section provides some of the basic background for the AASHO Road Test and is taken primarily from Highway Research Board's Special Report 61A, The AASHO Road Test: History and Description of the Project (1961). Location: Ottawa, Illinois The AASHO Road Test site (which eventually became part of I-80) at Ottawa, Illinois, was typical of northern climates (see Table 1). Table 1: AASHO Road Test Weather Average Mean Temperature (July) 24.5 C (76 o F) Average Mean Temperature (January) -2.8 C (27 o F) Annual Average Rainfall Average Depth of Frost (for fine-grained soil) 837 mm (34 inches) 711 mm (28 inches) Time Construction: August September 1958 Test Traffic: October November 1960 Special Studies: Spring and early summer 1961 Test Facilities Six 2-lane test loops (see Figure 1) Loop 1 = not subject to traffic, used to test environmental effects Loops 2 through 6 = subject to traffic described in Figure 2
2 Página 2 de 12 Test Tangent Flexible Prestressed Concrete Rigid Steel I- Beam Test Tangent Loop 5 Test Tangent Flexible Reinforced Concrete Rigid Steel I- Beam Test Tangent Loop 6 Figure 1: Loop 5 and 6 AASHO Road Test Layout (redrawn from Highway Research Board, 1961)
3 Página 3 de 12 Figure 2: Axle Weights and Distributions Used on Various Loops of the AASHO Road Test (redrawn from Highway Research Board, 1961) Performance Measurements The following measurements of performance were collected: Roughness and visual distress Deflections, strains, etc. Pavement Serviceability Index (PSI) Flexible Pavement Materials (Information for this section taken from Highway Research Board, 1962a and Highway Research Board, 1962b) The primary materials used in the flexible pavement sections will be briefly described below. This kind of information is helpful in comparing a particular project s set of materials to those used at the Road Test. HMA The HMA mixes used at the Road Test used:
4 Página 4 de 12 Crushed limestone coarse aggregate Natural siliceous coarse sand Mineral filler which was limestone dust Penetration grade asphalt cement ( pen) The gradation requirements for the surface and binder courses are given in Table 2. Table 2: AASHO Road Test HMA Gradation Requirements Sieve Surface Course Binder Course Gradation Limits Gradation Limits 1 in /4 in /2 in /8 in No No No No No No For the HMA surfaced test sections (in Loops 3-6), the surface course was 1.5 inches thick. The HMA mixes were designed by the Marshall method using 50 blows per face. The typical field asphalt contents were about 5.4 and 4.4 percent by weight of total mix for the surface and binder courses, respectively. The field air voids averaged 7.7 percent for the six test loops. Base Course The base course material was a crushed dolomitic limestone that conformed to the gradation range shown in Table 3. Table 3: AASHO Road Test Base Course Gradation Requirements Sieve Specification Range Actual Mean Percent Passing Percent Passing 1-1/2 in in /4 in /2 in No No No No No It is significant to note that 10 percent passed the mm (No. 200 sieve). Thus, the base was likely a bit frost susceptible. The CBR of the base material averaged percent based on laboratory tests; however, the test results ranged from a low of 52 percent to a high of 160 percent (total of 11 tests). The minimum specified CBR was 75 percent. Typical in-place mean dry densities were about 2242 to 2275 kg/m 3 (140 to 142 lb/ft 3), with mean moisture contents ranging from 5.6 to 6.1 percent. Subbase Course The subbase material was a sand-gravel mixture which conformed to the following gradation range shown in Table 4.
5 Página 5 de 12 Table 4: AASHO Road Test Subbase Course Gradation Requirements Specification Range Actual Mean Sieve Percent Passing Percent Passing 1-1/2 in in /4 in /2 in No No No No The CBR was specified not to exceed 60 percent. Typical laboratory CBR values ranged from 28 to 51 percent. The mean percent passing the mm (No. 200) sieve was 6.5 percent (a lesser percentage than the base course). Typical in-place mean dry densities ranged from 2227 to 2259 kg/m 3 (139 to 141 lb/ft 3 ), with moisture contents ranging from 6.1 to 6.8 percent. Subgrade One Road Test requirement was that all test pavements be built on a uniform embankment with the top 1 m (3 ft.) constructed of an A-6 soil. Tests on this soil revealed: LL = 31% PI = 16% P 200 = 82% γ dmax = 119 lb/ft 3 Optimum Water Content = 13% Field CBR and density tests on the completed embankment just prior to paving were (5.12): Average CBR = 2.9 CBR Range = Average Saturation = 85% Average Compaction = 98.5% Average Water Content = 13.8% Flexible Pavement Designs (Information for this section taken from Highway Research Board, 1962a and Highway Research Board, 1962b) The structural design portion of the AASHO Road Test flexible pavement experiment was designed as a full factorial experiment with the design factors being: surfacing thickness base thickness subbase thickness To accomplish the many different factorial combinations, the test loops were divided up into small test sections. Overall, there were 288 different flexible pavement test sections in the main experiments (332 counting replications).
6 Página 6 de 12 Each flexible pavement section in the main experiment was 30 m (100 ft.) long with all sections being separated by a transition pavement of at least 5 m (15 ft.) Table 5 summarizes the thicknesses for each loop. Table 5: AASHO Road Test Structural Design Thickness Summary Loop No. AC Thickness (in.) Base Thickness (in.) Subbase Thickness (in.)
7 Página 7 de 12 Flexible Pavement Performance Of the various axle loads applied to each of the test loops, a total of 1,114,000 load applications were made (not ESALs). Of the 332 test sections, 264 sections (or 80 percent) had reached a PSI of 1.5 or less on or before the end of the load application period (from November 1958 to June 1960). Tables 6 and 7 are used to overview the actual performance for Loops 4 and 6 (Loop 4 had an 18,000 lb single axle as one of its standard loads and Loop 6 had the heaviest axle loads used at the Road Test). Data from these two loops are shown because they are likely of the greatest contemporary interest. Table 6 shows that increasing AC thickness (from 3.0 to 5.0 in.) results in increased performance (number of loads until failure); however, not at as significant a rate as one might expect. Similar results are observed for Loop 6. Each section, if it reached a PSI of 1.5 prior to completion of all load applications (recall the total was 1,114,000 axle repetitions) was overlaid with new AC so that the trucks applying the loads could safely continue. For Loop 4, all of these overlays were applied during the months of March, April, and May. For Loop 6, 75 percent of the overlays were applied during March, April, and May. This suggests that freeze-thaw effects strongly influenced flexible pavement performance at the Road Test. The depth of freeze varied a bit from year-to-year but averaged about 28 in. for the flexible sections and generally reached 30 in. Such performance might provide additional insight into the required depth of pavement to resist freezethaw effects. Table 6: AASHO Road Test Loop 4 Results 2,3 Flexible Test Sections (after Highway Research Board, 1962b) Base and Subbase Thicknesses (in.) AC Thickness (in.) Axle ,000 lb single 2,000 72,000 98,000 74,000 82, ,000 80,000 92,000 (1.6) 32,000 lb tandem 12,000 74, ,000 76,000 86, ,000 80, , , ,000 lb single 78, , ,000 87, ,000 1,110,000 90,000 (1.9) (1.9) 32,000 lb tandem 83, , ,000 93, , , ,000 (2.0) (3.1) ,000 lb single 88, , , , , , ,000 (3.6) (3.3) Notes: 32,000 lb tandem 102, , , , ,000 (2.2) 678,000 (2.7) (2.7) 1. Replicate sections averaged 2. Values in parentheses are PSI at end of load applications 3. Values not in parentheses are the numbers of load applications to reach a PSI = 1.5 Table 7: AASHO Road Test Loop 6 Results Flexible Test Sections (after Highway Research Board, 1962b) Base and Subbase Thicknesses (in.) AC Thickness (in.) Axle ,000 lb single 72, , ,000 82,000 83, ,000 82, ,000 (2.0) 48,000 lb tandem 80, , , , , ,000 82, ,000 (2.0) ,000 lb single 78, , , , ,000 (1.8) 595, ,000 (3.3) 48,000 lb tandem 103, , , , , , , ,000 (3.5) ,000 lb single 141, , , ,000 (1.6) (3.2) 624,000 (2.4) (2.7) Notes: 48,000 lb tandem 579, ,000 (2.4) 250,000 (3.0) (3.9) (2.2) (2.6) (3.6) 1. Replicate sections averaged 2. Values in parentheses are PSI at end of load applications 3. Values not in parentheses are the numbers of load applications to reach a PSI = 1.5
8 Página 8 de 12 Tables 8 and 9 summarize information from Tables 6 and 7. Table 8: Loop 4 (18,000 lb Single Axle) Summary AC Thickness (in.) Poor Performance <500,000 reps Averaged Total Depth of Pavement (in.) and Percent of Frost Depth 1,2 Average Performance >500,000 reps Better Performance >1,114,000 reps (41%) 19.5 (65%) 21.0 (70%) (42%) 19.7 (65%) 20.0 (67%) (38%) 18.3 (61%) 21.0 (70%) Notes: 1. Frost depth = 30 in. 2. Load repetitions to a PSI of 1.5 (<500,000; >500,000) and load repetitions to greater than 1,114,000 (PSI > 1.5). Table 9: Loop 6 (30,000 lb Single Axle) Summary HMA Thickness (inches) Poor Performance <500,000 reps Averaged Total Depth of Pavement (in.) and Percent of Frost Depth 1,2 Average Performance >500,000 reps Better Performance >1,114,000 reps (67%) 27.5 (92%) 29.0 (97%) (61%) 25.3 (84%) 28.5 (95%) (64%) 26.3 (88%) 27.5 (92%) Notes: 1. Frost depth = 30 in. 2. Load repetitions to a PSI of 1.5 (<500,000; >500,000) and load repetitions to greater than 1,114,000 (PSI > 1.5). Based on the three categories of load repetitions (less than 500,000; more than 500,000; more than 1,114,000) from Tables 8 and 9, the total thickness of the base and subbase layers had a significant influence on the load repetitions. Given such information and the fact that most of the flexible sections which reached a PSI of 1.5 before completion of the Road Test traffic were overlaid immediately following the spring thaw (that is, the months of March, April, and May), then two preliminary observations are made: 1. For low ESAL pavements (say 500,000 ESALs or less as illustrated by Loop 4), the total depth of the pavement should be about 65 percent of the expected depth of frost. 2. For pavements subjected to much higher axle loads (say ESALs of about 5,000,000 or more) as illustrated by Loop 6 (recall the Load Equivalency Factor for a 30,000 lb single axle is about 8.0), the total depth of the pavement should be about 90 to 100 percent of the expected depth of frost. It is as yet uncertain as to whether such percentages as noted above apply to frost depths greater than say 30 in., since the evidence from the Road Test applies to a unique set of materials (base, subbase, and subgrade) and moisture conditions.
9 Página 9 de 12 Equivalent Single Axle Loads The design concept of the equivalent single axle load (ESAL) emerged from the AASHO road test and its volumes of data. Both the flexible and rigid ESAL equations and their corresponding calculated load equivalency factors (LEFs) are still used today in the 1993 AASHTO Guide. Although these equations and LEFs are reasonably accurate, a study conducted by Irick et al. (1991) for the Trucking Research Institute (TRI) reanalyzed the AASHO Road Test data with regard to estimation of LEFs. In general, the TRI study showed that LEFs for both flexible and rigid pavements should be larger for lighter loaded axles and smaller for heavier loaded axles as compared to AASHTO LEFs. Further, the LEFs for rigid pavements would be reduced for single axle loads greater than 80 kn (18,000 lb.) and tandem axle loads greater than 151 kn (34,000 lb.) as compared to AASHTO. The following LEFs from the TRI study and AASHTO illustrate these points: Table 10: TRI vs. AASHTO LEFs for Flexible and Rigid Pavements LEFs for p t = 2.5 Single Axle = 12,000 lb Single Axle = 30,000 lb Pavement Type SN TRI AASHTO TRI AASHTO Flexible Tandem Axle = 24,000 lb Tandem Axle = 48,000 lb Pavement Type SN or D TRI AASHTO TRI AASHTO Flexible Rigid 8.0-in. 9.5-in Thus, in general, for the heavier axle loads, the TRI study showed that single axle flexible LEFs would be somewhat higher than rigid LEFs. Tandem axle flexible and rigid LEFs would be about the same. Rigid Pavement Materials (Information for this section taken from Highway Research Board, 1962a and Highway Research Board, 1962b) The primary materials used in the rigid pavement sections will be briefly described below. This kind of information is helpful in comparing a particular project s set of materials to those used at the Road Test. Portland Cement Concrete Cement type = Type I Design cement content = 564 lb/yd 3 Design maximum water content = 5.3 gal/bag of cement (equates to a water-cement ratio of 0.47) Design strength (14 day cure): Minimum compressive strength = 3500 psi Minimum modulus of rupture (flexural strength) = 550 psi (using a third-point loading test)
10 Página 10 de 12 Design slump range: 1.5 to 2.5 in. Maximum aggregate sizes: 1.5 and 2.5 in. Linear coefficient of thermal expansion = 4.6 to 5.1 x 10-6 per F Table 11: Fresh PCC Parameters Parameter Maximum Aggregate Size 1.5 inch 2.5 inch Mean slump (inches) Mean air content (%) Mean cement content Table 12: Strength Properties Maximum Aggregate Size Age Compressive Strength (psi) 1.5 inch 2.5 inch Flexural Strength (psi) Compressive Strength (psi) Flexural Strength (psi) 3 days days days days year years Subbase Course The subbase course used beneath the PCC slabs was the same material as used for the subbase course in the flexible pavement sections. Subgrade The subgrade was the same as that under the flexible sections. Rigid Pavement Designs Overall, there were 260 rigid pavement test sections in the main experiment (312 counting replicates). Reinforced sections were 240 ft long with sawed, doweled transverse contraction joints spaced 40 ft apart. Non-reinforced sections were 120 ft long with sawed, doweled transverse contraction joints spaced 15 ft apart (no expansion joints). Dowel bar sizes varied with slab thickness. Reinforcement was welded steel fabric placed about 2 in. from the slab surface. Table 13 shows the various structural design parameters for each rigid pavement section.
11 Página 11 de 12 Table 13: Rigid Pavement Structural Design Parameters Loop No. PCC Slab Thickness (in.) Subbase Thickness (in.) Transverse Dowel Bars (Diameter x Length) 2.5 0, 6.0 3/8" x 12" , 6.0 5/8" x 12" 9.5 0, /4" x 18" , /8" x 18" 2.5 0, 3.0, 6.0 3/8" x 12" , 3.0, 6.0 1/2" x 12" 5.0 0, 3.0, 6.0 5/8" x 12" , 6.0, 9.0 1/2" x 12" , 6.0, 9.0 5/8" x 12" , 6.0, 9.0 7/8" x 18" , 6.0, 9.0 1" x 18" , 6.0, 9.0 5/8" x 12" , 6.0, 9.0 7/8" x 18" , 6.0, 9.0 1" x 18" , 6.0, /4" x 18" , 6.0, 9.0 7/8" x 18" , 6.0, 9.0 1" x 18" , 6.0, /4" x 18" , 6.0, /8" x 18" , 6.0, 9.0 1" x 18" , 6.0, /4" x 18" , 6.0, /8" x 18" , 6.0, /8" x 18" Rigid Pavement Performance Of the various axle loads applied to each of the test loops, a total of 1,114,000 load applications were made (not ESALs). Of the 312 rigid test sections, only 67 sections (or 21 percent) had reached a PSI of 1.5 or less at the end of the load application period (from November 1958 to June 1960). Tables 14 and 15 are used to overview the actual performance for Loops 4 and 6 (Loop 4 had an 18,000 lb single axle as one of its standard loads and Loop 6 had the heaviest axle loads used at the Road Test). Data from these two loops are shown because they are likely of the greatest contemporary interest. Table 14 reveals that the then standard axles caused failure in up to the 6.5 in. thick PCC slabs (8.0 in. and thicker slabs did not fail). For the heavier axles used in Loop 6, slabs up to 9.5 in. failed but 11 inch and thicker slabs did not fail. Further, subbase thickness did not seem to matter much. Table 14: AASHO Road Test Loop 4 Results 2,3 Rigid Test Sections (after Highway Research Board, 1962b) Subbase Thicknesses (in.) PCC slab Thickness (in.) Axle JPCP JRCP JPCP JRCP JPCP JRCP ,000 lb single 716, , , , , ,000 32,000 lb tandem 343, , , , , , ,000 lb single (3.8) (3.6) (4.3) (3.4) (3.0) (1.8) 32,000 lb tandem 687, ,000 1,000, , ,000 1,036, ,000 lb single (4.5) (3.9) (4.4) (3.9) (4.3) (4.3) 32,000 lb tandem (4.2) (4.0) (4.3) (3.8) (4.1) (4.2) Notes: 1. Replicate sections not shown 2. Values in parentheses are PSI at end of load applications 3. Values not in parentheses are the numbers of load applications to reach a PSI = 1.5.
12 Página 12 de 12 Table 15: AASHO Road Test Loop 6 Results 2,3 Rigid Test Sections (after Highway Research Board, 1962b) Subbase Thicknesses (in.) PCC Slab Axle JPCP JRCP JPCP JRCP JPCP JRCP Thickness (in.) ,000 lb single 878, ,000 (3.9) 974,000 (3.4) 768,000 48,000 lb tandem 618,000 (1.8) (4.1) 415,000 1,114, , ,000 lb single (3.6) (1.6) (4.3) (4.0) (4.2) (2.2) 48,000 lb tandem (3.1) (4.1) (4.3) (4.0) (4.3) 912, ,000 lb single (4.4) (4.4) (4.2) (4.3) (4.3) (4.2) 48,000 lb tandem (4.3) (4.4) (4.3) (4.2) (4.3) (4.1) ,000 lb single (4.2) (4.4) (4.0) (4.2) (4.2) (4.5) 48,000 lb tandem (4.3) (4.3) (4.2) (4.4) (4.4) (4.2) Notes: 1. Replicate sections not shown 2. Values in parentheses are PSI at end of load applications 3. Values not in parentheses are the numbers of load applications to reach a PSI = 1.5.
Roller-Compacted Concrete Pavement: Design and Construction Pavement Thickness esign and RCC-Pave Software Gregory E. Halsted, P.E. Pavements Engineer Portland Cement Association October 24, 2006 Atlanta,
F I N A L Construction Specifications for Keyhole Pavement Coring and Reinstatement Gas Technology Institute 1700 S. Mount Prospect Rd. Des Plaines, Illinois 60018 www.gastechnology.org Version 13 October
Final Report Evaluation of I-Pave Low Volume Road Design Software May 2015 Michael I Darter, William R. Vavrik, Dinesh Ayyala 2015 2014 Applied Research Associates, Inc. 1 Objectives 1. Obtain all documentation
Municipal Pavement Design with StreetPave Software March 5, 2009 Scott Haislip Senior VP Pavement Engineering Presentation Overview Background / history of the design procedure Concrete pavement design
Expected Service Life and Performance Characteristics of HMA Pavements in LTPP Expected Service Life and Performance Characteristics of HMA Pavements in LTPP Submitted to: Asphalt Pavement Alliance Prepared
SECTION 014500 QUALITY CONTROL PART 1 GENERAL 1.01 RELATED REQUIREMENTS A. Drawings and General Provisions of Contract, including General and Special Conditions and other Division 1 Specification Sections,
INITIAL COST COMPARISON OF RIGID AND FLEXIBLE PAVEMENTS: UNDER DIFFERENT TRAFIC AND SOIL CONDITIONS ABSTRACT T. Akakin Turkish Ready Mixed Concrete Association, Turkey email@example.com Y. Engin Turkish
SM 1110-02 Surfacing Manual INTRODUCTION Soil cement is a mixture of Portland Cement, a mineral soil (usually a graded sand) and water that is placed and compacted in one lift. It is an alternate to granular
Quality Assurance Program June 2005 2005 by Texas Department of Transportation (512) 416-2055 all rights reserved Quality Assurance Program June 2005 Manual Notices Manual Notice 2005-1To: Users of the
Issued 2005/06/01 Section 02742 Asphalt Concrete Pavement for Building Sites Page 1 of 8 PART 1 GENERAL 1.1 SECTION INCLUDES.1 Materials and installation for asphalt concrete pavement for car park areas,
Pavement Rehabilitation Using Hot Mix Asphalt - National Perspective - Rehabilitation Process Evaluate Existing Pavement and Conditions Evaluate Options Construct Project Monitor Performance Evaluate Existing
VIRGINIA DEPARMENT OF TRANSPORTATION MATERIALS DIVISION PAVEMENT DESIGN AND EVALUATION SECTION GUIDELINES FOR 1993 AASHTO PAVEMENT DESIGN FIRST PRINTING MAY 2000 REVISED OCTOBER 2001 REVISED JANUARY 2003
1.0 GENERAL 1.1 Scope 2.0 PRODUCTS 1.1.1 The asphaltic concrete shall consist of a homogeneous mixture of mineral aggregate, filler and asphaltic binder, combined in accordance with these Specifications.
INTRODUCTION TO CONCRETE PAVEMENTS Abstract Arvo Tinni Tinni Management Consulting February 2013 This paper describes the experiences and design methodologies for concrete pavements in Australia. It is
GUIDE FOR SPECIFYING ASPHALT PAVEMENTS FOR LOCAL GOVERNMENTS (USING INDOT STANDARD SPECIFICATIONS SECTION 402) This Guide incorporates the latest asphalt pavement technologies. It attempts to present the
SECTION 331 TYPE S ASPHALT CONCRETE 331-1 Description. Construct a Type S-I, Type S-II or Type S-III Asphalt Concrete as specified by the Contract. When offered as alternates, either Type may be constructed.
PART 1 GENERAL 1.1 SECTION INCLUDES SECTION 32 14 13.19 PERMEABLE INTERLOCKING CONCRETE PAVEMENT A. The requirements for construction of permeable interlocking concrete pavement: 1. Install the interlocking
ASPHALT CONCRETE MIXTURES Objectives: To introduce asphalt concrete To explain the asphalt concrete mixture To explain the types of asphalt concrete mixtures To explain the requirements of aggregates for
LTPP Lessons Learned: National Experiment March 14, 2013 Phoenix, AZ Jack Springer, P.E. FHWA Kevin Senn, P.E. NCE Lessons Learned Overview LTPP Program Benefits and Return on Investment Construction Effects
NORTH CENTRAL TEXAS COUNCIL OF GOVERNMENTS 17 TH ANNUAL PUBLIC WORKS ROUNDUP JUNE 8, 2016 Concrete Street Insanity Jerry Murawski, P.E. With Special Thanks to Jan Prusinski, P.E. Cement Council of Texas
Porous Pavement Alternatives Cost Analysis Prepared by Century West Engineering for Metro This cost analysis compares the construction costs of six different types of pavement for three different scenarios.
Quality control: Quality of the constructed work has been checked by our staff as per frequency and provision mentioned section 900 in MoRT&H and as per provision mentioned in Concession Agreement. The
STATE OF OHIO DEPARTMENT OF TRANSPORTATION SUPPLEMENT 1015 COMPACTION TESTING OF UNBOUND MATERIALS July 18, 2014 1015.01 General 1015.02 Definitions 1015.03 Referenced Standards 1015.04 Equipment 1015.05
Report No. CDOT-2012-11 Final Report APPLICATION OF ROLLER COMPACTED CONCR RETE IN COLORADO S ROADWAYS Nattapong Damrongwiriyanupapp Yu-Chang Liang Yunping Xi October 2012 COLORADOO DEPARTMENT OF TRANSPORTATION
Chapter 4 Bases 4-02 Gravel Base GEN 4-02.1 General Instructions Gravel Base is typically used in the construction of the roadway section and provides support for the pavement. For the pavement to provide
PART 1 GENERAL 1.1 SCOPE: A. This work consists of establishing the JMF for HMAC for use in road and street constructions and/or repairs. Once established and accepted the JMF will be used to determine
Abstract Testing and appraisal of polymer effect as an additive on asphalt mixture performance Hamid Sabbagh mollahosseini*,golazin Yadollahi**, Ershad Amoosoltani*** *, ***Executive of Engineering and
December 2014 CW 3110 SUB-GRADE, SUB-BASE AND BASE COURSE CONSTRUCTION TABLE OF CONTENTS 1. DESCRIPTION... 1 1.1 General... 1 1.2 Definitions... 1 1.3 Referenced Standard Construction Specifications...
TECH SUMMARY May 2011 Design of Concrete Overlays Using Existing Methodologies Authors Helga Torres Project Manager, The Transtec Group, Inc. 512-451-6233 firstname.lastname@example.org Robert Otto Rasmussen
Quality Assurance Concepts Peter C. Taylor Outline What is quality? Who cares? How do we get it? What is the important stuff? 1 Defining Quality Simple Definition (Philip Crosby) Quality: Conformance to
Standards for Specifying Construction Of Airports FAA Standard Materials in FAARFIELD Thickness Design Presented to: X ALACPA Seminar on Airport Pavements and VIII FAA Workshop By: David R. Brill. P.E.,
SPECIAL NOTE FOR ASPHALT WATERPROOFING MIX FOR BRIDGE-DECK OVERLAYS AND ADJACENT APPROACHES 1. DESCRIPTION. Asphalt Waterproofing Mix (AWM) is a highly elastomeric, polymermodified, impermeable asphalt
Technical Presentation: Follow up on HVS testing of Roller Compacted Concrete and Ultra-thin reinforced concrete test sections Louw du Plessis 12 Febuary 2015 Objectives UTRCP Previous round of HVS testing
APPENDIX B GUIDELINES FOR IDENTIFYING AND REPAIRING LOCALIZED AREAS OF DISTRESS IN AC PAVEMENTS PRIOR TO CAPITAL PREVENTIVE MAINTENANCE OR REHABILITATION REPAIRS I. Background Information A. AC Pavement
SECTION 02720 PART 1 - GENERAL 1.01 DESCRIPTION A. Section includes specifications for hot-mix asphalt concrete (HMAC) track underlayment and asphalt concrete (AC) paving. Track underlayment includes all
STATE OF OHIO DEPARTMENT OF TRANSPORTATION SUPPLEMENTAL SPECIFICATION 888 PORTLAND CEMENT CONCRETE PAVEMENT USING QC/QA October 21, 2011 888.01 General 888.02 Materials 888.03 Concrete Proportioning 888.04
CITY OF BRAMPTON LANDSCAPE SPECIFICATIONS SECTION 02743-1 PART 1 GENERAL 1.1 Related Work.1 All Division 1 Specification Sections.2 Section 01330 Submittals.3 Section 01450 Quality Control & Inspection.4
Brick Industry Association Flexible Vehicular Brick Paving A Heavy Duty Applications Guide Contents Foreword This Guide was prepared by the staff of the Brick Industry Association (BIA) with the assistance
State of the Art on Fiber Reinforced Concrete Recent Advances on the use of FRC for Pavement Design Presented to: 015 Concrete Pavements Plus Seminar Michael Mahoney, P.Eng. Director of Admixture and Fiber
TEXAS DEPARTMENT OF TRANSPORTATION What is ESAL? ESAL is the acronym for equivalent single axle load. ESAL is a concept developed from data collected at the American Association of State Highway Officials
Test Procedure for SOIL-CEMENT TESTING TxDOT Designation: Tex-120-E Effective Date: April 2013 1. SCOPE 1.1 This method consists of two parts. 1.1.1 Part I determines the unconfined compressive strength
CONSTRUCTION STANDARDS SECTION CS 5 ASPHALT CONCRETE CS 5-01 GENERAL: Furnishing, spreading and compacting Asphalt Concrete shall be in conformance with Section 39, Asphalt Concrete of the CALTRANS Standard
SECTION 34 32 38 ASPHALT PAVING PART 1 - GENERAL 1.01 DESCRIPTION A. Section includes specifications for hot-mix asphalt concrete (HMAC) track underlayment and asphalt concrete (AC) paving. Track underlayment
Long Life Concrete Pavement Joint Performance Joint Rehabilitation Gary Fick, Trinity Construction Management Services, Inc. Representing the National CP Tech Center Driving Forces for Concrete Pavement
High-Speed Nondestructive Testing and Intelligent Construction Systems 1st International Conference on Transportation Construction Management February 9-11, 9 2008 Orlando, Florida Ted Ferragut, P.E. NDT
Software Development (PAKPAVE) for Flexible Pavement Design Rafi Ullah Khan, Muhammad Imran Khan and Afed Ullah Khan Abstract In today s world, the road and surface failure of the flexible pavement has
MEPDG Work Plan Task No. 8: Validation of Pavement Performance Curves for the Mechanistic-Empirical Pavement Design Guide Final Report February 2009 Sponsored by Iowa Department of Transportation (CTRE
Pak. J. Engg. & Appl. Sci. Vol., July, 22 (p. 6-65) Rutting Based Evaluation of Asphalt Mixes Kamran Muzaffar Khan, Mumtaz Ahmed Kamal 2. Associate Professor, Civil Engg. Department, University of Engg.
SECTION 32 14 13.19 PERMEABLE INTERLOCKING CONCRETE PAVEMENT (1995 MasterFormat Section 02795) Note: This guide specification for U.S. applications describes construction of permeable interlocking concrete
SCHEDULE OF GOVERNING ITEMS OF WORK OF THE DPWH STANDARD SPECIFICATIONS FOR HIGHWAYS, BRIDGES AND AIRPORTS, 1998, (VOLUME II) PART C - EARTHWORK Item 100 - Clearing & Grubbing None Item 101 - Removal of
PLACEMENT AND CONSTRUCTION OF CEMENT TREATED SUBGRADESOIL CEMENT BASE COURSE 311.1 DESCRIPTION: This item shall consist of a cement treated subgrade base course composed of a mixture of local soil, portland
FWD/HWD Void Detection Beneath Concrete Pavements or Overlaid Concrete Pavements SWIFT 2010 Calgary, AB Presentation Outline Voids what s the big deal? What causes them? How can we detect them? Oops Development
L. Huang, A.M. Sha*, F. Ma, Z.Z. Liu and X.L. Zou Chang an University, China August 3, 2015 ISSAEST, Fairbanks, AK, USA, August 2-5, 2015 The national or local standards of the asphalt stabilized aggregates
Revised 09-06-3, WKS Datasheet No. 7.6a & 7.6b MOHAWK COLLEGE OF APPLIED ARTS AND TECHNOLOGY BUILDING AND CONSTRUCTION SCIENCES DEPARTMENT Flexural Strength of Concrete (The Modulus of Rupture Test) INTRODUCTION
Ohio Department of Transportation Division of Production Management Office of Geotechnical Engineering Geotechnical Bulletin GB 1 PLAN SUBGRADES Geotechnical Bulletin GB1 was jointly developed by the Offices
PAVEMENT REHABILITATION using BITUMEN STABILISATION STATE OF THE ART 23 rd Road Pavement Forum Fern Hill Hotel, Tweedie, KZN Wednesday 9 th May 2012 Dave Collings UCD Technology LOUDON INTERNATIONAL THE
Modern Techniques for Concrete Pavement Design Robert Rodden, P.E. Director of Technical Services & Product Development American Concrete Pavement Association km of Paved Roadway by Country 5.000.000 4.500.000
Specification Guidelines: Allan Block Modular Retaining Wall Systems The following specifications provide Allan Block Corporation's typical requirements and recommendations. At the engineer of record's
Louisiana Case Study: Implementation of CRM Binder in PG specification. AASHTO Subcomittee on Materials Biloxi, Mississippi August 4-10, 2012 Chris Abadie, P.E. My Story Background Approach Phase I Evaluation:
CEMENT AND LIME STABILIZATION OF SUBGRADE SOILS (07-12-07) DB5 R21 General The Design-Build Team shall be responsible for the following: Sampling 1. Performing all laboratory tests in a laboratory certified
4. Subgrade : Foundation Considerations 1. Introduction The performance of any structure is strongly dependent on the foundations. Road pavements are no exceptions and their foundations need to be fundamentally
STP 208-7 Standard Test Procedures Manual Section: MIX DESIGN BY SHORT- CUT METHOD 1. SCOPE 1.1. Description of Test This method describes the Portland Cement Association short-cut procedure for determining
HIGHWAYS DEPARTMENT GUIDANCE NOTES ON ROAD SURFACE REQUIREMENTS FOR EXPRESSWAYS AND HIGH SPEED ROADS Research & Development Division RD/GN/032 June 2007 1. Purpose ROAD SURFACE REQUIREMENTS FOR EXPRESSWAYS
Pavement Design for Rural Low Volume Roads Using Cement and Lime Treatment Base General Manager, Pavement, Material and Geotechnical Division, Intercontinental Consultants and Technocrats Private Limited,
University of Pittsburgh Rehabilitation Strategies for Bonded Concrete Overlays of Asphalt Pavements Authors: J. M Vandenbossche S. Sachs August 2013 1. Introduction Bonded concrete overlays of asphalt
304.06 DIVISION 300 BASES SECTION 304 AGGREGATE BASE COURSE DESCRIPTION 304.01 This work consists of furnishing and placing one or more courses of aggregate and additives, if required, on a prepared subgrade.
CLASS II BASE COURSE - Section 302 Class II Base Courses are similar to Class I Base Courses, with the exception that placement on a subgrade layer built in accordance with Specification Section 305 is
Raad et al. 1 FIELD AGING EFFECTS ON THE FATIGUE OF ASPHALT CONCRETE AND ASPHALT-RUBBER CONCRETE by Lutfi Raad. Professor of Civil Engineering Director, Transportation Research Center University of Alaska
SECTION 02795 UNI PERMEABLE INTERLOCKING CONCRETE PAVEMENT Note: This guide specification is intended for use in the U.S. It describes construction of permeable interlocking concrete pavers on a permeable,
Design and Construction of Roller-Compacted Concrete Pavements for Container Terminals David R. Luhr PhD PE * Program Manager, Portland Cement Association, PO Box 5895, Cary, NC 27511; PH 919-462-0840;
ITEM 247 FLEXIBLE BASE 247.1. Description. Construct a foundation course composed of flexible base. 247.2. Materials. Furnish uncontaminated materials of uniform quality that meet the requirements of the
The Production and Use of Recycled Concrete in the USA Thomas Van Dam, Ph.D., P.E., FACI Principal Engineer CTL Group Introduction In the United States, concrete is the most commonly used recycled material
Permeable Interlocking Concrete Pavements The Stormwater Problem 1 Stormwater Management Objectives Water Quantity Accommodate water volumes & peak flows Water Quality Control pollutant levels A Low Impact
11 Soils Field Procedures Using the Sand Cone Method Apparatus Cone Correction and Bulk Density Factors Procedure CHAPTER ELEVEN: SOILS FIELD PROCEDURES USING THE SAND CONE METHOD Field density determination